J. Phys. Chem. A 2010, 114, 1247–1254 1247Vibrationally Resolved Photoelectron Spectroscopy of Di-Gold Carbonyl ClustersAu 2 (CO) n - (n ) 1-3): Experiment and Theory †Yi-Lei Wang, ‡ Hua-Jin Zhai, § Lu Xu, ‡ Jun Li,* ,‡ and Lai-Sheng Wang* ,§,|Department of Chemistry & Key Laboratory of Organic Optoelectronics and Molecular Engineering ofMinistry of Education, Tsinghua UniVersity, Beijing 100084, China, Department of Physics, Washington StateUniVersity, 2710 UniVersity DriVe, Richland, Washington 99354, and Chemical & Materials Sciences DiVision,Pacific Northwest National Laboratory, MS K8-88, P.O. Box 999, Richland, Washington 99352ReceiVed: April 17, 2009; ReVised Manuscript ReceiVed: July 31, 2009We report vibrationally resolved photoelectron spectroscopy (PES) of Au 2 (CO) n - (n ) 1-3), in combinationwith relativistic density functional theory (DFT) and ab initio calculations. The ground-state transition in thespectrum of Au 2 CO - is broad, containing vibrational structures both in the bending and in the CO stretchingmodes and suggesting a large structural change from Au 2 CO - to Au 2 CO. The ground-state transitions forboth n ) 2 and 3 display a well-resolved vibrational progression in the CO stretching mode with frequenciesof 2110 ( 40 and 2160 ( 40 cm -1 , respectively. The PES data show that chemisorption of the first two CO’seach induces a significant red-shift in the electron binding energies. The third CO is physisorbed, inducingonly a slight increase in electron binding energies relative to Au 2 (CO) 2 - . Relativistic DFT and ab initiocalculations are performed to determine the ground-state structures for Au 2 (CO) n - and Au 2 (CO) n , and theresults agree well with the experiment. Au 2 (CO), Au 2 (CO) 2 , and Au 2 (CO) 2 - are all found to be linear, whileAu 2 (CO) - is bent due to the Renner-Teller effect. A strong spin-orbit effect is found in Au 2 (CO) 2 - thatquenches the Renner-Teller effect, keeping the linear structure for this anion. The physisorption in Au 2 (CO) 3-is borne out in CCSD(T) calculations. However, a wide range of DFT methods tested fail to correctly predictthe relative energies of the physisorbed versus chemisorbed isomers for Au 2 (CO) 3 - .1. IntroductionCatalysis of highly dispersed gold nanoparticles has been arapidly expanding field since the pioneering work by Harutaand co-workers. 1 Despite extensive state-of-the-art surfaceinvestigations over the past 20 years, 2-18 the mechanisms ofthe highly useful catalytic reactions involving gold are not wellunderstood. 1,19 Gas-phase studies of CO and O 2 adsorption onsize-selected Au clusters have emerged as an alternativeapproach to provide insight into the mechanisms of catalyticCO oxidation. 20-49 Experimental and theoretical studies haveestablished that O 2 adsorbs molecularly on certain goldclusters. 20-23 Coadsorption of CO and O 2 on small gold clusterswas also observed, in which CO and O 2 were shown to adsorbcooperatively. 24,25The interaction of CO with gold clusters has been the subjectof numerous studies, and saturation adsorption of CO on goldclusters has been observed. 24,29-37 Infrared spectra of Au-COcomplexes in neon matrix have led to the identifications of+AuCO, Au(CO) 2 ,Au 2 (CO) 2 ,Au n (CO) (n ) 2-5), and Au(CO) n(n ) 1-4). 31,34 Vibrational spectroscopy on size-elected Au m -(CO) + n and Au m (CO) - n clusters has also been reported. 35,37 Theadsorption energies of CO on gold cluster cations Au + n (n )1-65) have been determined in a radiative association kineticsstudy, ranging from 1.1 eV for smaller clusters to 0.65 eV forlarger ones. 36 However, the electronic and structural propertiesof CO-Au - n clusters remain poorly understood. We reported† Part of the “W. Carl Lineberger Festschrift”.* Corresponding author. E-mail: email@example.com; firstname.lastname@example.org.‡ Tsinghua University.§ Washington State University and Pacific Northwest National Laboratory.| Permanent address: Department of Chemistry, Brown University, 324Brook Street, Providence, RI 02912.previously photoelectron spectroscopy (PES) of several seriesof gold carbonyl cluster anions, Au m (CO) n - (m ) 2-5, n )1-7). 50 We observed that adsorption of the first few CO’sinduces significant red-shifts to the PES spectra. For each goldcluster, CO adsorption reaches a critical number, beyond whichfurther CO adsorption hardly changes the spectra. The criticalCO number corresponds exactly to the available low-coordinateapex sites in the corresponding bare Au clusters. We suggestedthat CO first chemisorbs to the apex sites and additional CO’sonly physisorb to the chemisorption-saturated Au-CO complexes.In subsequent studies on the Au 6 (CO) n - (n ) 1-9)complexes, 51,52 we observed that the first three CO’s chemisorbto the three apex sites of the triangular Au 6 - cluster. Startingfrom the adsorption of the fourth CO, significant structuralchanges occur for the Au 6 - cluster such that it can chemisorbup to six CO’s, whereas additional CO’s are physisorbed.In the current Article, we report a combined experimentaland theoretical study on a series of di-gold carbonyl clusters:Au 2 (CO) n - and Au 2 (CO) n (n ) 1-3). Higher resolution PESspectra are obtained at 532 nm (2.331 eV), yielding vibrationalinformation and more accurate electron detachment energies.The adsorption of the first two CO’s each decreases significantlythe electron binding energies, whereas the third CO is physisorbed,inducing a slight increase in the electron bindingenergies. The ground-state detachment transitions are vibrationallyresolved in the CO stretching mode with frequenciesof 2110 ( 40 and 2160 ( 40 cm -1 , respectively, for Au 2 (CO) 2and Au 2 (CO) 3 . The CO frequency in Au 2 (CO) 2 is substantiallyred-shifted with respect to bare CO (2143 cm -1 ), while that inAu 2 (CO) 3 is slightly blue-shifted. The latter is unexpected andmay provide interesting insights into the nature of surfaceAu-CO species. 13,53-62 We have performed DFT and ab initio10.1021/jp903558v © 2010 American Chemical SocietyPublished on Web 09/18/2009
1248 J. Phys. Chem. A, Vol. 114, No. 3, 2010 Wang et al.calculations including scalar relativistic and spin-orbit (SO)coupling effects for Au 2 (CO) n - and Au 2 (CO) n . The ground stateof Au 2 (CO) - is found to be considerably bent with a Au-C-Obond angle of 133°, whereas Au 2 (CO) is linear. Both Au 2 (CO) 2-and Au 2 (CO) 2 are shown to be linear. All DFT methods usedare shown to be inadequate for the Au 2 (CO) 3 - complex. OnlyCCSD(T) calculations predict the physisorbed Au 2 (CO) 3 - isomerto be the ground state, consistent with the experimentalobservation.2. Experimental and Computational Methods2.1. Photoelectron Spectroscopy. The experiment was carriedout using a magnetic-bottle PES apparatus equipped witha laser vaporization supersonic cluster source, the details ofwhich have been described elsewhere. 63 -Briefly, the Au m (CO) ncluster anions were produced by laser vaporization of a puregold target in the presence of a helium carrier gas seeded with2% CO. Various Au m (CO) - n clusters were generated andanalyzed using a time-of-flight mass spectrometer. TheAu 2 (CO) - n (n ) 0-3) species of current interest were eachmass-selected and decelerated before being photodetached.Under our experimental conditions, only relatively weak masssignals were observed for the Au 2 (CO) - n species, whereas nomass signals were observed for the Au(CO) - n series. Theseobservations suggest that Au - and Au - 2 are probably lessreactive with CO than the larger clusters, consistent withprevious experiments on chemical reactivity of gold clusteranions. 21,24,30,33 PES spectra were measured at 532 nm (2.331eV). Photoelectrons were collected at nearly 100% efficiencyby the magnetic bottle and analyzed in a 3.5 m long electronflight tube. The PES spectra were calibrated using the knownspectra of Rh - , and the energy resolution of the apparatus was∆E k /E k ≈ 2.5%, that is, ∼25 meV for 1 eV electrons.2.2. Computational Methods. DFT calculations were performedusing the PW91 functional of the generalized gradientapproximation (GGA) implemented in the Amsterdam DensityFunctional program (ADF 2007.01). 64 The uncontracted Slaterbasis sets with the quality of triple-ζ plus two polarizationfunctions (TZ2P) were used, with the frozen core approximationapplied to the [1s 2 -4f 14 ] core for Au and the [1s 2 ] cores forboth C and O. 65 The scalar relativistic (SR) and SO couplingeffects were taken into account by the zero-order-regularapproximation (ZORA). 66 Geometries were optimized at the SRlevel, and single-point energy calculations were performed atthe SO level. Vibrational frequency calculations were carriedout to verify that the species are minima on the potential energysurface. Vertical electron detachment energies (VDEs) wereobtained at the anion geometry by using a combined ∆SCF-TDDFT approach, 67 where the first VDE was calculated fromthe difference of the ground-state energy of the anions andneutrals (i.e., ∆SCF) and the higher VDEs were calculated fromthe ground-state energy of the anions and the excited-stateenergies of the neutrals by using TDDFT. To better describethe neutral excited states, the SAOP (statistical average of orbitalpotentials) functional was also used to do TDDFT calculations,where all-electron basis sets were applied for all of the atoms.Because of the complicated nature of the delicate electroncorrelations in the gold and CO interactions, 41 ab initio wavefunction theory calculations at the coupled-cluster level with singleand double and perturbative triple excitations [CCSD(T)] 68 werealso performed for n ) 0-2 using the MOLPRO 2008 program 69to assess the accuracy of the DFT results. We used a relativistic19-valence-electron pseudopotential (ECP60MDF) 70 and the augcc-pVTZ-PPbasis sets 71 (11s10p9d3f2g)/[6s6p5d3f2g] for gold andaug-cc-pVTZ basis sets for carbon and oxygen, 72 denoted asAVTZ hereafter. The SO coupling effect was included by usinga state-interacting method 73 with spin-orbit pseudopotentialsat the complete active space self-consistent field (CASSCF) 74level of theory, and SO-free energies were replaced by thosefrom CCSD(T) calculations. Because the proper selection ofactive spaces is crucial to state-averaged CASSCF calculations,we included all of the 5d and 6s orbitals for Au 2 in the activespace with all 22 electrons in 12 active orbitals being correlated,that is, CASSCF(22e, 12o). For Au 2 (CO) and Au 2 (CO) 2 , largesizeactive spaces including the 5d and 6s orbitals of Au andthe frontier π and π* orbitals of CO were adopted, that is,CASSCF(26e, 16o) for Au 2 (CO) and CASSCF(30e, 19o) forAu 2 (CO) 2 . Based on the contributions of the orbitals in theseactive spaces to the concerned states, the following spaces werechosen to reduce the computational cost of the subsequentcalculations: CASSCF(6e, 6o) for Au 2 (CO) and CASSCF(18e,13o) for Au 2 (CO) 2 . The occupations of the natural orbitals agreewith each other within 0.01 and 0.002, respectively, for Au 2 (CO)and Au 2 (CO) 2 between the two types of active spaces. Additionally,the first excited energies calculated using the twotypes of active spaces are the same for Au 2 (CO), indicating thesmaller active space is appropriate. The states relevant to thefirst excitation were included in the state-averaged CASSCF,with the following states being selected on the basis of ourTDDFT results: 1 Σ g , 3 Π u , and 3 Σ u for Au 2 , 1 A′ and 3 A′ forAu 2 (CO), and 1 Σ g and 3 Π u for Au 2 (CO) 2 .Because the PW91 method turned out to have large errorsfor Au 2 (CO) - 3 , we further performed DFT calculations usinghybrid functionals of B3LYP and TPSSh, and GGA functionalof PW91, using the NWChem 5.0 program. 75 On the basis ofthe optimized TPSSh geometries, ab initio calculations werefurther carried out at the CCSD(T) level using MOLPRO 2008.In these calculations, we used the same AVTZ basis sets asbefore. Basis sets superposition error (BSSE) was corrected withthe counterpoise method 76 using Au - 2 and CO’s as fragments.3. Experimental ResultsThe PES spectra of Au 2 (CO) - n (n ) 0-3) at two detachmentphoton energies are shown in Figure 1. The 193 nm spectra(Figure 1a), which revealed more electronic transitions, werereported previously 50 and are included here for comparison withthe 532 nm data and the theoretical calculations. The mainobservations from the 193 nm data were that the first two CO’seach induce a significant red-shift for the electron bindingenergies of the ground-state transition (X) by ∼0.5-0.7 eV,whereas the third CO induces a slight blue-shift (0.17 eV) (Table1). The second PES band (A) was observed at roughly constantbinding energies (3.9-4.2 eV), causing the X-A energy gaps(i.e., the HOMO-LUMO gaps of the corresponding neutralclusters) to increase as a function of CO from 2.00 f 2.55 f3.26 f 3.35 eV for Au 2 (CO) - n (n ) 0-3) (Table 1).The 532 nm spectra (Figure 1b) only allowed the groundstatetransition to be observed and were significantly betterresolved with vibrational structures in each case. We reportedthe 532 nm spectrum of Au - 2 in our previous study of Au 2 H - . 77It displays a vibrational progression with a spacing of 190 (15 cm -1 , which agrees with a prior high resolution spectrum. 78The Au 2 (CO) - spectrum appears to be rather broad, andvibrational structures were not well resolved except for a hintof the 1 r 0 transition for CO stretching at ∼1.75 eV. Thebroad spectrum indicates a large anion-to-neutral structurechange and the involvement of multiple vibrational modes. Thus,the adiabatic electron detachment energy (ADE) for Au 2 (CO) -
Di-Gold Carbonyl Clusters Au 2 (CO) n - (n ) 1-3) J. Phys. Chem. A, Vol. 114, No. 3, 2010 1249Figure 2. Optimized structures of Au 2 (CO) n and Au 2 (CO) n - (n ) 0-2)at the DFT/PW91 level. Bond lengths are in angstroms.Figure 3. Optimized structures of Au 2 (CO) 3 and Au 2 (CO) - 3 at theDFT/PW91 level. Bond lengths are in angstroms.Figure 1. Photoelectron spectra of Au 2 (CO) n - (n ) 0-3) at (a) 193nm (6.424 eV) and (b) 532 nm (2.331 eV). Energy gaps betweenfeatures X and A for each species are labeled. Vertical bars indicatethe resolved vibrational structures.TABLE 1: Observed Adiabatic (ADE) and Vertical (VDE)Detachment Energies, Energy Gaps, and VibrationalFrequencies from the Photoelectron Spectra of Au 2 (CO) n - (n) 0-3)ADE(eV) a∆ADE(eV) bVDE (eV) aband X band AX-A gap(eV) cvib. freq.(cm -1 ) a,d-Au 2 1.94 (2) e 2.01 (2) 4.01 (2) 2.00 190 (15) eAu 2 (CO) - 1.25 (5) f -0.69 1.50(3) 4.05 (2) 2.55Au 2 (CO) - 2 0.69 (3) -0.56 0.69 (3) 3.95 (3) 3.26 2110 (40)Au 2 (CO) - 3 0.86 (3) 0.17 0.86 (3) 4.21 (2) 3.35 2160 (40)a Numbers in parentheses represent experimental uncertainties inthe last digits. b ∆ADE ≡ ADE [Au 2 (CO) n - ] - ADE [Au 2 -(CO) n-1 - ], which characterizes the influence of the nth CO moleculeto the electron binding energies of Au 2 (CO) n - . c Evaluated from theVDE difference between bands X and A. d Ground-state vibrationalfrequencies of the corresponding neutral species. e More accurateADE (1.938 ( 0.007 eV) and vibrational frequency (190.9 cm -1 )were reported previously (ref 78). f Because of the large geometrychange between the anion and neutral, this number should beconsidered as a threshold value, which represents the upper limit ofthe true ADE.(1.25 eV, Table 1) estimated from the leading edge of the broadspectrum should be considered as a threshold value, whichrepresents the upper limit for the true ADE. In contrast, thespectra of Au 2 (CO) 2 - and Au 2 (CO) 3 - each exhibit a wellresolvedvibrational progression with spacings of 2110 ( 40and 2160 ( 40 cm -1 , respectively, which should correspond tothe CO stretch. The ADE and VDE for both the n ) 2 and 3species can be accurately determined from the intense and sharp0-0 peak in the corresponding spectrum, as given in Table 1.The weak broad feature at ∼1.5 eV in the 532 nm spectrumof Au 2 (CO) - 2 (Figure 1b), which is also discernible in the 193nm (Figure 1a), has binding energies similar to the spectrum ofAu 2 (CO) - -. It is likely due to photofragmentation, Au 2 (CO) 2+ hν f Au 2 (CO) - + CO, followed by photodetachment of theAu 2 (CO) - product. The weak feature at ∼3.6 eV in the 193nm spectrum of Au - 2 (Figure 1a) was identified to come fromthe Au 2 H - impurity previously. 77 There are also visible weakfeatures between the X and A bands in the 193 nm spectra ofAu 2 (CO) - n (n ) 1-3), which were likely due to minorimpurities.4. Theoretical ResultsThe optimized structures at PW91 level are shown in Figure2 for Au 2 (CO) - n and Au 2 (CO) n (n ) 0-2), and those for n )3 are in Figure 3. We calculated a variety of possible geometriesfor Au 2 (CO) - ,Au 2 (CO) - 2 , and their neutrals. In the lowestenergy structures, CO is found to coordinate to Au 2 terminallyvia the C atom. The lowest energy structure of Au 2 (CO) - ( 2 A′,Figure 2e) is bent with C s symmetry, whereas Au 2 (CO) - 2 ( 2 Π u ,Figure 2f) is linear with D ∞h symmetry. Both Au 2 (CO) ( 1 Σ) andAu 2 (CO) 2 ( 1 Σ g ) neutrals are linear with C ∞V and D ∞h symmetries,respectively. Our result for the bent Au 2 (CO) - agrees withseveral previous DFT calculations. 38-41 Our linear Au 2 (CO)structure also agrees with two previous calculations. 39,41For Au 2 (CO) - 3 and Au 2 (CO) 3 , we performed PW91 geometryoptimizations on many possible structures including mixed
1250 J. Phys. Chem. A, Vol. 114, No. 3, 2010 Wang et al.TABLE 2: Calculated PW91 Adiabatic (ADE) and Vertical (VDE) Detachment Energies and Energy Gaps for Au 2 (CO) n - (n )0-3), and Vibrational Frequencies of the Corresponding Neutral Species aVDE (eV)X-A gap (eV)ADE (eV) ∆ADE (eV) b feature X feature A PW91 SAOP CCSD(T) vib. freq. (cm -1 ) c-Au 2 1.94 2.01 3.48 1.47 1.67 1.96 177Au 2 (CO) - 1.19 -0.75 1.77 3.40 1.63 1.71 2.49 2093-Au 2 (CO) 2 1.06 -0.13 1.17 3.73 2.56 2.45 3.23 2095-dAu 2 (CO) 3 1.20 0.15 1.30 3.82 2.52 2095, 2119a The X-A gaps at the SAOP and CCSD(T) levels are also included. All quantities were calculated with SO corrections except thevibrational frequencies, for which only scalar-relativistic effects were included. b See footnote b in Table 1. c Ground-state vibrationalfrequencies of the corresponding neutral species. For the CO complexes, the frequency refers to the CO stretch. d Isomer I (Figure 3b). Thecorresponding data for isomer II (Figure 3d): ADE (1.55 eV), VDE (1.74 eV), and X-A gap (1.24 eV).chemisorption-physisorption complexes and all-CO-chemisorbedstructures. The two low-lying structures are shown inFigure 3, where isomer I of Au 2 (CO) - 3 (C s , 2 A′) contains aphysisorbed CO lying aslant above the linear Au 2 (CO) - 2 core.In isomer II (C s , 2 A′′), all three CO’s are chemisorbed with oneAu atom coordinated by two CO’s. For the anions, PW91calculations predict isomer II to be 0.48 eV lower in energythan isomer I. For the Au 2 (CO) 3 neutral, PW91 predicts isomerII (C s , 1 A′′) to be more stable than isomer I (C s , 1 A′) by 0.13eV. However, the calculated VDEs and simulated PES spectrumfrom isomer II of Au 2 (CO) - 3 do not agree with the experiment(see footnote d in Table 2). Thus, further DFT and ab initiocalculations were performed to evaluate the relative energiesbetween isomers I and II for Au 2 (CO) - 3 . With ZPE (zero-pointenergy) and SO corrections, the PW91, B3LYP, and TPSShmethods using the AVTZ basis sets erroneously predict thatisomer II is lower in energy than isomer I by 0.46, 0.10, and0.31 eV, respectively. While the BSSE correction is only 0.003eV with TPSSh, it becomes as large as 0.16 eV with CCSD(T)/AVTZ. As a result, CCSD(T) single-point energy calculationswith ZPE, BSSE, and SO corrections correctly predict thatisomer I is lower in energy than isomer II by about 0.02 eV.Note that the two near-degenerate states of Au 2 (CO) - 3 (isomerI) derived from the 2 Π u ground state of Au 2 (CO) - 2 are within0.04 eV at the CCSD(T)/VTZ level of theory.-The adsorption energies of the first and second CO to Au 2are -1.03 and -0.94 eV, respectively. These adsorption energiesreveal that the adsorption of the first CO does not prevent theadsorption of the second CO and the first two CO’s have similarbinding strengths to those of the Au - 2 core. When the twoterminal sites are used up, the third CO becomes physisorbedwith a rather small adsorption energy of -0.19 eV. Thistheoretical result is consistent with our previous observation thatCO prefers apex sites on small Au - n clusters. 50-52The calculated electronic properties for Au 2 (CO) - n andAu 2 (CO) n at the PW91 level are summarized in Table 2.Apparently, PW91 underestimates the energy gaps by 0.5-0.9eV. Such deviation is far larger than expected, prompting us tocompute the energy gaps using the SAOP and CCSD(T)methods (Table 2). While the SAOP results show no improvementas compared to the PW91 data, the CCSD(T) results indeedagree well with the experiment.5. Comparison between Experiment and TheoryAs shown in Table 2, the PW91 ADE (1.94 eV) and the firstVDE (2.01 eV) for Au - 2 are in quantitative agreement with thecorresponding experimental values (Table 1). However, thePW91 VDE for the first excited band A (3.48 eV) is lower by0.53 eV relative to the experimental value (4.01 eV), resultingin a much smaller PW91 X-A gap. For Au 2 (CO) - , the PW91Figure 4. Contour surfaces (isosurface value ) 0.04 au) of the frontierorbitals of Au 2 (CO) n (n ) 0-2).ADE (1.19 eV) and VDE (1.77 eV) agree well with theexperimental values (Table 1). Again, the PW91 VDE for bandA (3.40 eV) is much lower relative to the experimental value(4.05 eV). For Au 2 (CO) 2 - , the PW91 ADE (1.06 eV) and thefirst VDE (1.17 eV) are both too high relative to the experimentby 0.37 and 0.48 eV, respectively. For Au 2 (CO) 3 - , the PW91ADE (1.20 eV) and the first VDE (1.30 eV) for the physisorbedisomer (Figure 3b) are also too high, but the deviation (0.34and 0.44 eV) relative to the experiment is similar to those forAu 2 (CO) 2 - . However, the PW91 ADE and the first VDE forthe chemisorbed isomer II (Figure 3d) totally disagree with theexperiment (see footnote d in Table 2) and thus can be ruledout to be responsible for the observed spectra of Au 2 (CO) 3 - .As mentioned above, the PW91 VDE for the first excitedstate band A is all significantly underestimated, resulting insmaller X-A gaps for all Au 2 (CO) n - (n ) 1-3) species. Thedeviation from experiment is -0.53 eV for Au 2 - and variesbetween -0.70 and -0.92 eV for Au 2 (CO) n - (n ) 1-3). Thevalence molecular orbitals for neutral Au 2 (CO) n (n ) 0-2) areshown in Figure 4. The LUMO’s for Au 2 (CO) and Au 2 (CO) 2are mainly CO π* orbitals, and their HOMO’s mainly involveaAu 2 σ orbital. The X-A gap is equivalent to promote a Au 2σ electron to the CO π* orbital, that is, a metal-to-ligand charge
Di-Gold Carbonyl Clusters Au 2 (CO) n - (n ) 1-3) J. Phys. Chem. A, Vol. 114, No. 3, 2010 1251transfer transition. It is known that TDDFT tends to underestimateexcitation energies of charge-transfer transitions, 79 explainingwhy the errors of the PW91 X-A gaps for Au 2 (CO) n-(n ) 1-3) are much more severe as compared to that for Au - 2 .To further investigate the large PW91 deviations of the X-Agaps, CCSD(T) and SAOP calculations were performed forAu 2 (CO) n (n ) 0-2). Au 2 (CO) 3 was omitted in these calculationsbecause the nature of its electronic transition to the firstexcited state is similar to that of Au 2 (CO) 2 due to thephysisorbed nature of the third CO. The CCSD(T) X-A gapsare also shown in Table 2, and they are in quantitative agreementwith the experiment. However, the overall performance of theasymptotically corrected SAOP (Table 2) functional is no betterthan PW91.The structural changes between the anions and neutral COcomplexesare also consistent with the experimental observations.The Au 2 (CO) - anion is bent with a ∠AuCO angle of 133°(Figure 2e), while the ground state of Au 2 (CO) is linear (Figure2b), which explains the broad ground-state PES band. The CObond length is also slightly shortened from Au 2 (CO) - toAu 2 (CO) by 0.042 Å, consistent with the observation of COstretch in the 532 nm spectrum (Figure 1b). The large differencebetween the calculated ADE and VDE for Au 2 (CO) - reflectsthe large structural changes upon electron detachment. ForAu 2 (CO) - 2 and the physisorbed Au 2 (CO) - 3 , there is very littlestructure change upon electron detachment. The main differenceis the slight shortening of the CO bond length, consistent withthe simple CO stretching progression observed in the 532 nmspectra of Au 2 (CO) - 2 and Au 2 (CO) - 3 (Figure 1b). Again, the-difference between the calculated ADE and VDE for Au 2 (CO) 2and Au 2 (CO) - 3 is also very small, in line with the smallstructural change upon electron detachment. The simple COvibrational progression observed in the 532 nm spectrum ofAu 2 (CO) - 3 can also rule out the chemisorbed isomer II becausethere are more significant structural changes between the anionand the neutral (Figure 3c and d). The calculated CO stretchingfrequencies for Au 2 (CO) n at the PW91 level are 2093 cm -1 forn ) 1, 2095 cm -1 for n ) 2, and 2095 and 2119 cm -1 for n )3 (Table 2). Considering the complexity of the Au-COsystem, 13,80,81 the agreement between the computed and experimentalfrequencies is reasonable.Overall, the theoretical results are in good agreement withthe experiment, lending considerable credence to the structuresidentified for Au 2 (CO) - n and Au 2 (CO) n (n ) 1-3).6. Discussion6.1. Au 2 (CO) - and Au 2 (CO) - 2 : Renner-Teller Effectversus Spin-Orbit Effect. The decrease of electron bindingenergies upon CO chemisorption to Au - 2 in the Au 2 (CO) - n (n) 1-2) complexes is quite unusual, suggesting strong chemicalinteractions. The molecular orbitals shown in Figure 4 allow aqualitative understanding of this trend. The LUMO of Au 2 isan antibonding σ orbital. The terminal coordination of CO toAu 2 in the linear complexes would significantly destabilize thisorbital. Consequently, the LUMO’s of Au 2 (CO) and Au 2 (CO) 2become the unoccupied CO π* orbitals, which are much higherlying relative to the LUMO of Au 2 . Occupation of these highlying CO-centered LUMO’s by the extra electron in theAu 2 (CO) - n anions would result in reduced electron bindingenergies relative to the bare Au - 2 .In the linear structure, occupation of the doubly degenerateLUMO would lead to doubly degenerate electronic states: 2 Πfor Au 2 (CO) - and 2 Π u for Au 2 (CO) - 2 . In these linear anions,the degenerate electronic states are unstable against bendingvibrations, resulting in the Renner-Teller (RT) effect that woulddistort the linear structures and lift the electronic degeneracy. 82The RT effect is similar to the Jahn-Teller effect for nonlinearmolecules. The bent structure of Au 2 (CO) - is entirely aconsequence of the RT effect. However, the RT effect does notseem to occur in Au 2 (CO) - 2 : our optimized structure for thisanion with SO effect remains linear, in agreement with thesimple vibrational progression in the 532 nm PES spectrum.Our analysis showed that the 4π u LUMO of Au 2 (CO) 2 contains19% Au 6p and 3% Au 5d characters, leading to a SO splittingenergy of 0.20 eV, which is larger than the RT effect (0.16eV). Thus, the RT effect is quenched and the anion remainslinear as a result of the strong SO effect. A similar analysisrevealed that the 6π LUMO orbital of Au 2 (CO) contains 15%Au 6p and 8% Au 5d character. Because the Au 6p orbitalshave a large SO effect, less Au 6p character results in less SOsplitting (0.09 eV) for Au 2 (CO) - -as compared to Au 2 (CO) 2(0.20 eV). The calculated RT energy is 0.67 eV for Au 2 (CO) - ,much larger than the SO splitting energy for Au 2 (CO) - . Hence,the RT effect dominates in Au 2 (CO) - , leading to the bentstructure. There is a previous report of a bent Au 2 (CO) - 2 , 40which is problematic because of the neglect of the SO effect.It is noteworthy that in the bent Au 2 (CO) - structure the singlyoccupied orbital has weaker σ-donation from CO and aconsiderable Au-Au σ* character like in the Au - 2 anion.Consequently, the Au-Au bond lengths in these two anionsare both lengthened by more than 0.1 Å as compared to thecorresponding neutrals. On the contrary, in Au 2 (CO) - 2 theexcess electron is located in the neutral LUMO, which has asmall σ-bonding character between the two gold atoms due tothe D ∞h symmetry. Therefore, the Au-Au bond length of theAu 2 (CO) - 2 anion is smaller than that of the neutral by 0.014Å.6.2. Comparison between DFT and ab Initio Methods forAu 2 (CO) - 3 : Physisorption versus Chemisorption. The experimentalPES spectra of Au 2 (CO) - 3 are similar to those ofAu 2 (CO) - 2 (Figure 1), suggesting that the third CO inAu 2 (CO) - 3 is physisorbed to a Au 2 (CO) - 2 core. However, atthe PW91 level of theory, the chemisorbed isomer II (Figure3d) is predicted to be the lowest in energy for Au 2 (CO) - 3 , butits calculated first VDE (1.74 eV), second VDE (2.98 eV), andenergy gap (1.24 eV) deviate considerably from the experiment(first VDE, 0.86 eV; second VDE, 4.21 eV; energy gap, 3.35eV). Furthermore, one of the Au atoms in this isomer iscoordinated by two CO ligands, which is inconsistent with thegeneral observation that each low-coordinate Au atom can onlychemisorb one CO ligand at low CO coverage. 50-52 It is knownthat DFT methods can carry large errors in predicting relativeenergies of isomers with significantly different geometries orphysiochemical interactions. 83 Indeed, single-point CCSD(T)calculations show that the physisorbed isomer I is more stableby ∼0.02 eV, suggesting the PW91 calculations carry a large-error (at least 0.5 eV) for the relative energies for the Au 2 (CO) 3isomers. This is not totally surprising considering the complicatednature of Au-CO interactions and the weak interactionsinvolving the physisorbed CO. We also note that the popularB3LYP, PW91, and TPSSh methods with SO corrections alsoincorrectly predict that isomer II is 0.10, 0.46, and 0.31 eV,respectively, lower in energy.In isomer I of Au 2 (CO) - 3 (Figure 3b), the distance betweenthe C atom of the physisorbed CO and the middle point of thetwo Au atoms is 3.342 Å, and the C ···Au distance is 3.575 Å.This C ···Au distance is much larger than the sum of the atomicradius, indicating only weak van der Waals interactions between
1252 J. Phys. Chem. A, Vol. 114, No. 3, 2010 Wang et al.the third CO and Au 2 . Treating such weak interactions is still achallenging bottleneck for DFT methods, suggesting the importanceof accurate experimental data and the interplay ofcombined experimental and theoretical efforts.6.3. Au 2 (CO) 2 and Au 2 (CO) 3 : Classical versus NonclassicalAu(0)-CO Complexes. The 532 nm spectra of Au 2 (CO) 2-and Au 2 (CO) - 3 (Figure 1b) represent the only species for whichit is possible to resolve a CO stretching progression among allAu m (CO) - n (m ) 2-6; n ) 1-9) complexes that we haveinvestigated. 50-52 Relative to free CO molecule (vibrationalfrequency: 2143 cm -1 ), the vibrational frequency of Au 2 (CO) 2(2110 cm -1 ) is red-shifted, making the Au 2 (CO) 2 complex a“classical” carbonyl species. In contrast, the vibrational frequencyof Au 2 (CO) 3 (2160 cm -1 ) is slightly blue-shifted relativeto free CO, making it a “nonclassical” carbonyl species. 37,84Chemical bonding in transition metal carbonyl complexes(M-CO) comprises MrCO σ donation and MfCO π backdonation:CO is both a σ-donor and a π-acceptor ligand. 84 TheCO stretching frequency is a useful indicator of the magnitudeof σ- and π-bonding in metal carbonyls. In classical M-COtransition metal complexes, strong MfCO π back-donationweakens the CO bond, resulting in a red-shift in the COstretching frequency. However, strong σ donation or weak πback-donation can lead to stronger CO bonding and an increasedCO stretching frequency in nonclassical M-CO complexes.Surface studies show that CO stretching in Au(0)-CO speciesis at ∼2110 cm -1 , 53-62 where the red-shift relative to free COmolecule is small. Our current observation of a CO stretchingfrequency of 2110 cm -1 in Au 2 (CO) 2 is in excellent agreementwith the surface results. Our observed CO stretching inAu 2 (CO) 2 falls between those observed for Au m (CO) + n andAu m (CO) - n from gas-phase IR spectroscopy. 35Au-CO complexes are rare, but it is generally believed thatσ donation is important in Au-CO complexes, whereas π backdonationis negligible, making them nonclassical carbonylcomplexes. This usually involves a Au + center. 37,84 However, anonclassical Au(0)-CO species has not been reported in theliterature. 31,34,53-62 The Au 2 (CO) 3 complex represents an exampleof nonclassical Au(0)-CO species. Although our measuredfrequencies (2160 cm -1 ) carry large uncertainties, the relativelylarge CO vibrational spacing in the 532 nm spectrum ofAu 2 (CO) - 3 in comparison to that of Au 2 (CO) - 2 is quite obvious(Figure 1b). The CO stretching frequencies in Au 2 (CO) 2 andAu 2 (CO) 3 differ by as large as 50 cm -1 , despite the fact thatthe third CO in Au 2 (CO) - 3 and Au 2 (CO) 3 is shown to interactweakly with the chemisorbed Au 2 (CO) 2 core (Figure 3a andb), suggesting that the weakly bonded CO influences theinteractions of the terminal CO with gold. As shown in Figure3a, the physisorbed CO is in a bridging position and weaklyinteracts with both Au atoms. It is conceivable that the weakCO-Au 2 interactions withdraw net charge from the Au 2 core,thus strengthening the COfAu σ donation and weakening theAufCO π back-donation for the terminal CO’s.The active Au species in gold catalysts have been assignedon the basis of the observed CO frequencies as follows:Au(0)-CO (2105-2120 cm -1 ), Au δ+ -CO (2130, 2145 cm -1 ),Au(I)-CO (2160-2170 cm -1 ), and Au(III)-CO (>2170cm -1 ). 13,54-62 However, two recent benchmarking theoreticalworks on the simplest AuCO complex 41,81 showed the complexityof the Au-CO system, suggesting that the equilibriumgeometry, the adsorption energies, and in particular the COvibrational frequency are all challenging properties to calculatefor the current approximate methods. In this context, gas-phasevibrational information such as that obtained from the currentstudy is valuable both in helping resolve the controversy insurface studies and in calibrating the computational methods.For example, numerous surface studies have shown Au carbonylspecies with CO frequencies between 2150 and 2170 cm -1 , andtheir assignments have been inconsistent and controversial. 54-58Freund and co-workers 57 reported an intriguing surface carbonylspecies at 2165 cm -1 , which appeared at higher or saturatedCO exposure. It corresponds to a more weakly bound COrelative to those on Au(0) sites and is assigned to CO bound toextremely small Au clusters with Au + character, inconsistentwith the common notion that cationic Au absorbs CO morestrongly. In light of our current observation, it is conceivablethat nonclassical Au(0)-CO complexes with physisorbed COmay be relevant to the surface IR data.7. ConclusionsWe report a combined experimental and theoretical study ofa series of gas-phase di-gold carbonyl clusters, Au 2 (CO) - n (n) 1-3). Photoelectron spectroscopy shows that adsorption ofthe first two CO’s each induces a significant red-shift in theelectron binding energies (0.69 and 0.56 eV) and the third COonly induces a slight blue-shift (0.17 eV), indicating a chemisorption-to-physisorptiontransition from n ) 2ton ) 3inAu 2 (CO) - n . The ground-state detachment transitions forAu 2 (CO) - 2 and Au 2 (CO) - 3 are vibrationally resolved, yieldingvibrational frequencies of 2110 ( 40 and 2160 ( 40 cm -1 forthe neutral Au 2 (CO) 2 and Au 2 (CO) 3 clusters, respectively. TheAu 2 (CO) 3 species represents a nonclassical Au(0)-CO complexand may be relevant to surface carbonyl species under high COcoverage. DFT calculations at the PW91 level are carried outto determine the structures of Au 2 (CO) - n and Au 2 (CO) n (n )1-3). Both Au 2 (CO) and Au 2 (CO) 2 are found to be linearmolecules with CO coordinated to Au terminally via C.However, Au 2 (CO) - is found to be bent due to the Renner-Tellereffect, whereas strong spin-orbit effects in Au 2 (CO) - 2 quenchthe Renner-Teller effect to remain linear. Au 2 (CO) - 3 is foundto be a physisorbed complex, in which the third CO is onlyweakly interacting with a linear Au 2 (CO) - 2 core. Both pureGGA and hybrid DFT methods are found to be inadequate topredict the relative energies for the CO physisorption versuschemisorption in Au 2 (CO) - 3 . CCSD(T) calculations have to beused, showing that the physisorption isomer is the ground state,in agreement with the experimental observation.Acknowledgment. The experimental work was supported bythe National Science Foundation (CHE-0749496) and performedat the W. R. Wiley Environmental Molecular Sciences Laboratory,a national scientific user facility sponsored by the Departmentof Energy’s Office of Biological and EnvironmentalResearch and located at the Pacific Northwest National Laboratory,operated for DOE by Battelle. The theoretical work wassupported by NKBRSF (2006CB932305, 2007CB815200) andNSFC (20525104, 20933003) in China. The calculations wereperformed using a HP Itanium2 cluster at Tsinghua NationalLaboratory for Information Science and Technology andShanghai Supercomputing Center.Supporting Information Available: Complete refs 69 and75 and Cartesian coordinates for Au 2 (CO) n and Au 2 (CO) n - (n) 0-3) clusters at the PW91 level of theory. This material isavailable free of charge via the Internet at http://pubs.acs.org.References and Notes(1) For selected recent reviews, see: (a) Haruta, M. Catal. Today 1997,36, 153. (b) Haruta, M. Chem. Rec. 2003, 3, 75. (c) Bond, G. C.; Thompson,
Di-Gold Carbonyl Clusters Au 2 (CO) n - (n ) 1-3) J. Phys. Chem. A, Vol. 114, No. 3, 2010 1253D. T. Catal. ReV.-Sci. Eng. 1999, 41, 319. (d) Meyer, R.; Lemire, C.;Shaikhutdinov, Sh. K.; Freund, H.-J. Gold Bull. 2004, 37, 72. (e) Kung,M. C.; Davis, R. J.; Kung, H. H. J. Phys. Chem. C 2007, 111, 11767.(2) (a) Valden, M.; Lai, X.; Goodman, D. W. Science 1998, 281, 1647.(b) Chen, M. S.; Goodman, D. W. Science 2004, 306, 252. (c) Chen, M. S.;Kumar, D.; Yi, C. W.; Goodman, D. W. Science 2005, 310, 291.(3) (a) Sanchez, A.; Abbet, S.; Heiz, U.; Schneider, W. D.; Häkkinen,H.; Barnett, R. N.; Landman, U. J. Phys. Chem. A 1999, 103, 9573. (b)Yoon, B.; Häkkinen, H.; Landman, U.; Wirz, A. S.; Antonietti, J. M.; Abbet,S.; Judai, K.; Heiz, U. Science 2005, 307, 403.(4) (a) Kim, T. S.; Stiehl, J. D.; Reeves, C. T.; Meyer, R. J.; Mullins,C. B. J. Am. Chem. Soc. 2003, 125, 2018. (b) Stiehl, J. D.; Kim, T. S.;McClure, S. M.; Mullins, C. B. J. Am. Chem. Soc. 2004, 126, 1606.(5) (a) Wahlstrom, E.; Lopez, N.; Schaub, R.; Thostrup, P.; Ronnau,A.; Africh, C.; Lægsgaard, E.; Norskov, J. K.; Besenbacher, F. Phys. ReV.Lett. 2003, 90, 026101. (b) Matthey, D.; Wang, J. G.; Wendt, S.; Matthiesen,J.; Schaub, R.; Lægsgaard, E.; Hammer, B.; Besenbacher, F. Science 2007,315, 1692.(6) Fu, Q.; Saltsburg, H.; Flytzani-Stephanopoulos, M. Science 2003,301, 935.(7) Guzman, J.; Gates, B. C. J. Am. Chem. Soc. 2004, 126, 2672.(8) Date, M.; Okumura, M.; Tsubota, S.; Haruta, M. Angew. Chem.,Int. Ed. 2004, 43, 2129.(9) Lemire, C.; Meyer, R.; Shaikhutdinov, S.; Freund, H.-J. Angew.Chem., Int. Ed. 2004, 43, 118.(10) Lee, S.; Fan, C.; Wu, T.; Anderson, S. L. J. Am. Chem. Soc. 2004,126, 5682.(11) Deng, X.; Min, B. K.; Guloy, A.; Friend, C. M. J. Am. Chem. Soc.2005, 127, 9267.(12) (a) Hughes, M. D.; Xu, Y. J.; Jenkins, P.; McMorn, P.; Landon,P.; Enache, D. I.; Carley, A. F.; Attard, G. A.; Hutchings, G. J.; King, F.;Stitt, E. H.; Johnston, P.; Griffin, K.; Kiely, C. J. Nature 2005, 437, 1132.(b) Enache, D. I.; Edwards, J. K.; Landon, P.; Solsona-Espriu, B.; Carley,A. F.; Herzing, A. A.; Watanabe, M.; Kiely, C. J.; Knight, D. W.; Hutchings,G. J. Science 2006, 311, 362. (c) Herzing, A. A.; Kiely, C. J.; Carley, A. F.;Landon, P.; Hutchings, G. J. Science 2008, 321, 1331.(13) (a) Sterrer, M.; Yulikov, M.; Risse, T.; Freund, H.-J.; Carrasco, J.;Illas, F.; Di Valentin, C.; Giordano, L.; Pacchioni, G. Angew. Chem., Int.Ed. 2006, 45, 2633. (b) Sterrer, M.; Yulikov, M.; Fischbach, E.; Heyde,M.; Rust, H. P.; Pacchioni, G.; Risse, T.; Freund, H.-J. Angew. Chem., Int.Ed. 2006, 45, 2630.(14) Hayden, B. E.; Pletcher, D.; Suchsland, J. P. Angew. Chem., Int.Ed. 2007, 46, 3530.(15) Turner, M.; Golovko, V. B.; Vaughan, O. P. H.; Abdulkin, P.;Berenguer-Murcia, A.; Tikhov, M. S.; Johnson, B. F. G.; Lambert, R. M.Nature 2008, 454, 981.(16) (a) Liu, Z. P.; Hu, P.; Alavi, A. J. Am. Chem. Soc. 2002, 124,14770. (b) Liu, Z. P.; Gong, X. Q.; Kohanoff, J.; Sanchez, C.; Hu, P. Phys.ReV. Lett. 2003, 91, 266102. (c) Liu, Z. P.; Jenkins, S. J.; King, D. A.Phys. ReV. Lett. 2005, 94, 196102.(17) Lopez, N.; Janssens, T. V. W.; Clausen, B. S.; Xu, Y.; Mavrikakis,M.; Bligaard, T.; Norskov, J. K. J. Catal. 2004, 223, 232.(18) (a) Molina, L. M.; Hammer, B. Phys. ReV. Lett. 2003, 90, 206102.(b) Molina, L. M.; Hammer, B. J. Chem. Phys. 2005, 123, 161104. (c)Molina, L. M.; Lesarri, A.; Alonso, J. A. Chem. Phys. Lett. 2009, 468,201.(19) Cho, A. Science 2003, 299, 1684.(20) Cox, D. M.; Brickman, R.; Creegan, K.; Kaldor, A. Z. Phys. D1991, 19, 353.(21) Lee, T. H.; Ervin, K. M. J. Phys. Chem. 1994, 98, 10023.(22) Salisbury, B. E.; Wallace, W. T.; Whetten, R. L. Chem. Phys. 2000,262, 131.(23) (a) Stolcic, D.; Fischer, M.; Gantefor, G.; Kim, Y. D.; Sun, Q.;Jena, P. J. Am. Chem. Soc. 2003, 125, 2848. (b) Kim, Y. D.; Fischer, M.;Gantefor, G. Chem. Phys. Lett. 2003, 377, 170. (c) Sun, Q.; Jena, P.; Kim,Y. D.; Fischer, M.; Gantefor, G. J. Chem. Phys. 2004, 120, 6510.(24) (a) Hagen, J.; Socaciu, L. D.; Elijazyfer, M.; Heiz, U.; Bernhardt,T. M.; Wöste, L. Phys. Chem. Chem. Phys. 2002, 4, 1707. (b) Socaciu,L. D.; Hagen, J.; Bernhardt, T. M.; Wöste, L.; Heiz, U.; Häkkinen, H.;Landman, U. J. Am. Chem. Soc. 2003, 125, 10437. (c) Hagen, J.; Socaciu,L. D.; Heiz, U.; Bernhardt, T. M.; Wöste, L. Eur. Phys. J. D 2003, 24,327.(25) Wallace, W. T.; Whetten, R. L. J. Am. Chem. Soc. 2002, 124, 7499.(26) (a) Kimble, M. L.; Castleman, A. W., Jr.; Mitric, R.; Bürgel, C.;Bonacic-Koutecky, V. J. Am. Chem. Soc. 2004, 126, 2526. (b) Kimble,M.; Moore, N. A.; Johnson, G. E.; Castleman, A. W., Jr.; Bürgel, C.; Mitric,R.; Bonacic-Koutecky, V. J. Chem. Phys. 2006, 125, 204311. (c) Bürgel,C.; Reilly, N. M.; Johnson, G. E.; Mitric, R.; Kimble, M. L.; Castleman,A. W., Jr.; Bonacic-Koutecky, V. J. Am. Chem. Soc. 2008, 130, 1694. (d)Johnson, G. E.; Reilly, N. M.; Tyo, E. C.; Castleman, A. W., Jr. J. Phys.Chem. C 2008, 112, 9730.(27) Veldeman, N.; Lievens, P.; Andersson, M. J. Phys. Chem. A 2005,109, 11793.(28) Zhai, H. J.; Bürgel, C.; Bonacic-Koutecky, V.; Wang, L. S. J. Am.Chem. Soc. 2008, 130, 9156.(29) Nygren, M. A.; Siegbahn, P. E. M.; Jin, C.; Guo, T.; Smalley, R. E.J. Chem. Phys. 1991, 95, 6181.(30) (a) Wallace, W. T.; Whetten, R. L. J. Phys. Chem. B 2000, 104,10964. (b) Wallace, W. T.; Wyrwas, R. B.; Leavitt, A. J.; Whetten, R. L.Phys. Chem. Chem. Phys. 2005, 7, 930.(31) Liang, B.; Andrews, L. J. Phys. Chem. A 2000, 104, 9156.(32) Luttgens, G.; Pontius, N.; Bechthold, P. S.; Neeb, M.; Eberhardt,W. Phys. ReV. Lett. 2002, 88, 076102.(33) Balteanu, I.; Balaj, O. P.; Fox, B. S.; Beyer, M. K.; Bastl, Z.;Bondybey, V. E. Phys. Chem. Chem. Phys. 2003, 5, 1213.(34) (a) Jiang, L.; Xu, Q. J. Phys. Chem. A 2005, 109, 1026. (b) Xu,Q.; Jiang, L. J. Phys. Chem. A 2006, 110, 2655.(35) (a) Fielicke, A.; von Helden, G.; Meijer, G.; Pedersen, D. B.;Simard, B.; Rayner, D. M. J. Am. Chem. Soc. 2005, 127, 8146. (b) Fielicke,A.; von Helden, G.; Meijer, G.; Simard, B.; Rayner, D. M. J. Phys. Chem.B 2005, 109, 23935.(36) (a) Neumaier, M.; Weigend, F.; Hampe, O.; Kappes, M. M. J. Chem.Phys. 2005, 122, 104702. (b) Neumaier, M.; Weigend, F.; Hampe, O.;Kappes, M. M. J. Chem. Phys. 2006, 125, 104308. (c) Neumaier, M.;Weigend, F.; Hampe, O.; Kappes, M. M. Faraday Discuss. 2008, 138, 393.(37) Velasquez, J., III.; Njegic, B.; Gordon, M. S.; Duncan, M. A. J.Phys. Chem. A 2008, 112, 1907.(38) Häkkinen, H.; Landman, U. J. Am. Chem. Soc. 2001, 123, 9704.(39) Wu, X.; Senapati, L.; Nayak, S. K.; Selloni, A.; Hajaligol, M.J. Chem. Phys. 2002, 117, 4010.(40) Yuan, D. W.; Zeng, Z. J. Chem. Phys. 2004, 120, 6574.(41) Schwerdtfeger, P.; Lein, M.; Krawczyk, R. P.; Jacob, C. R. J. Chem.Phys. 2008, 128, 124302.(42) (a) Varganov, S. A.; Olson, R. M.; Gordon, M. S.; Meitu, H.J. Chem. Phys. 2003, 119, 2531. (b) Varganov, S. A.; Olson, R. M.; Gordon,M. S.; Mills, G.; Meitu, H. Chem. Phys. Lett. 2003, 368, 778. (c) Mills, G.;Gordon, M. S.; Meitu, H. Chem. Phys. Lett. 2002, 359, 493.(43) Yoon, B.; Häkkinen, H.; Landman, U. J. Phys. Chem. A 2003, 107,4066.(44) (a) Ding, X. L.; Li, Z. Y.; Yang, J. L.; Hou, J. G.; Zhu, Q. S.J. Chem. Phys. 2004, 120, 9594. (b) Ding, X. L.; Dai, B.; Yang, J. L.;Hou, J. G.; Zhu, Q. S. J. Chem. Phys. 2004, 121, 621.(45) McKenna, K. P.; Shluger, A. L. J. Phys. Chem. C 2007, 111, 18848.(46) Mitric, R.; Bürgel, C.; Bonacic-Koutecky, V. Proc. Natl. Acad. Sci.U.S.A. 2007, 104, 10314.(47) Prestianni, A.; Martorana, A.; Ciofini, I.; Labat, F.; Adamo, C. J.Phys. Chem. C 2008, 112, 18061.(48) Torres, M. B.; Fernandez, E. M.; Balbas, L. C. J. Phys. Chem. A2008, 112, 6678.(49) (a) An, W.; Pei, Y.; Zeng, X. C. Nano Lett. 2008, 8, 195. (b) Gao,Y.; Shao, N.; Bulusu, S.; Zeng, X. C. J. Phys. Chem. C 2008, 112, 8234.(50) Zhai, H. J.; Wang, L. S. J. Chem. Phys. 2005, 122, 051101.(51) Zhai, H. J.; Kiran, B.; Dai, B.; Li, J.; Wang, L. S. J. Am. Chem.Soc. 2005, 127, 12098.(52) Zhai, H. J.; Pan, L.-L.; Dai, B.; Kiran, B.; Li, J.; Wang, L. S. J.Phys. Chem. C 2008, 112, 11920.(53) Worz, A. S.; Heiz, U.; Cinquini, F.; Pacchioni, G. J. Phys. Chem.B 2005, 109, 18418.(54) Yates, D. J. C. J. Colloid Interface Sci. 1969, 29, 194.(55) Lee, J. Y.; Schwank, J. J. Catal. 1986, 102, 207.(56) Guillemot, D.; Borovkov, V. Yu.; Kazansky, V. B.; Polisset-Thfoin,M.; Fraissard, J. J. Chem. Soc., Faraday Trans. 1997, 93, 3587.(57) Lemire, C.; Meyer, R.; Shaikhutdinov, S. K.; Freund, H.-J. Surf.Sci. 2004, 552, 27.(58) Centeno, M. A.; Hadjiivanov, K.; Venkov, Tz.; Klimev, Hr.;Odriozola, J. A. J. Mol. Catal. A 2006, 252, 142.(59) Tadayyoni, M. A.; Weaver, M. J. Langmuir 1986, 2, 179.(60) Boccuzzi, F.; Chiorini, A.; Tsubota, S.; Haruta, M. J. Phys. Chem.1996, 100, 3625.(61) Maciejewski, M.; Fabrizioli, P.; Grunwaldt, J. D.; Becker, O. S.;Baiker, A. Phys. Chem. Chem. Phys. 2001, 3, 3846.(62) Karpenko, A.; Leppelt, R.; Plzak, V.; Behm, R. J. J. Catal. 2007,252, 231.(63) (a) Wang, L. S.; Cheng, H. S.; Fan, J. J. Chem. Phys. 1995, 102,9480. (b) Wang, L. S.; Wu, H. In AdVances in Metal and SemiconductorClusters. IV. Cluster Materials; Duncan, M. A., Ed.; JAI Press: Greenwich,CT, 1998; pp 299-343.(64) ADF 2007.01, SCM, Theoretical Chemistry, Vrije Universiteit,Amsterdam, The Netherlands (http://www.scm.com). (a) te Velde, G.;Bickelhaupt, F. M.; Baerends, E. J.; Guerra, C. F.; van Gisbergen, S. J. A.;Snijders, J. G.; Ziegler, T. J. Comput. Chem. 2001, 22, 931. (b) Guerra,C. F.; Snijders, J. G.; te Velde, G.; Baerends, E. J. Theor. Chem. Acc. 1998,99, 391.(65) van Lenthe, E.; Baerends, E. J. J. Comput. Chem. 2003, 24, 1142.(66) van Lenthe, E.; Baerends, E. J.; Snijders, J. G. J. Chem. Phys. 1993,99, 4597.
1254 J. Phys. Chem. A, Vol. 114, No. 3, 2010 Wang et al.(67) Li, J.; Li, X.; Zhai, H. J.; Wang, L. S. Science 2003, 299, 864.(68) (a) Purvis, G. D.; Bartlett, R. J. J. Chem. Phys. 1982, 76, 1910. (b)Scuseria, G. E.; Janssen, C. L.; Schaefer, H. F. J. Chem. Phys. 1988, 89,7382.(69) Werner, H.-J.; MOLPRO, Version 2008.1, a package of ab initioprograms; see: http://www.molpro.net.(70) Figgen, D.; Rauhut, G.; Dolg, M.; Stoll, H. Chem. Phys. 2005, 311,227.(71) Peterson, K. A.; Puzzarini, C. Theor. Chem. Acc. 2005, 114, 283.(72) Dunning, T. H., Jr. J. Chem. Phys. 1989, 90, 1007.(73) Berning, A.; Schweizer, M.; Werner, H.-J.; Knowles, P. J.; Palmieri,P. Mol. Phys. 2000, 98, 1823.(74) (a) Roos, B. O.; Taylor, P. R.; Siegbahn, P. E. M. Chem. Phys.1980, 48, 157. (b) Roos, B. O. Int. J. Quantum Chem. 1980, S14, 175.(75) Bylaska, E. J.; NWChem, A Computational Chemistry Package forParallel Computers, Version 5.0; Pacific Northwest National Laboratory,Richland, WA 99352-0999, 2006.(76) Boys, S. F.; Bernardi, F. Mol. Phys. 1970, 19, 553.(77) Zhai, H. J.; Kiran, B.; Wang, L. S. J. Chem. Phys. 2004, 121, 8231.(78) Ho, J.; Ervin, K. M.; Lineberger, W. C. J. Chem. Phys. 1990, 93,6987.(79) Dreuw, A.; Weisman, J. L.; Head-Gordon, M. J. Chem. Phys. 2003,119, 2943.(80) Bagus, P. S.; Pacchioni, G. J. Phys. Conf. Ser. 2008, 117, 012003.(81) Giordano, L.; Carrasco, J.; Di Valentin, C.; Illas, F.; Pacchioni, G.J. Chem. Phys. 2006, 124, 174709.(82) Renner, R. Z. Phys. 1934, 92, 172.(83) Pan, L. L.; Li, J.; Wang, L. S. J. Chem. Phys. 2008, 129, 024302.(84) (a) Rack, J. J.; Strauss, S. H. Catal. Today 1997, 36, 99. (b) Strauss,S. H. J. Chem. Soc., Dalton Trans. 2000, 1.JP903558V